In situ synthesis of silver nanoparticles on the surface of PDMS with high antibacterial activity and biosafety toward an implantable medical device
© The Author(s) 2017
Received: 7 September 2017
Accepted: 3 November 2017
Published: 27 November 2017
We developed a straightforward method to fabricate antibacterial silicon films via the in situ synthesis of silver nanoparticles (AgNPs) on a polydimethylsiloxane (PDMS) film. To grow AgNPs attached on the film, AgNP seeds were synthesized through the reduction of silver ions electrostatically bound to hydroxyl groups formed on the surface of the film after treatment with air plasma. In the growth reaction, silver ions were reduced on the seeds of AgNPs by sodium citrate in a solution of AgNO3, which allowed for the formation of AgNPs with sizes of up to ~ 500 nm, which The formed AgNPs on the films were characterized using UV–vis spectrophotometer, scattering electron microscope and induced coupled mass spectrometer. The amount of AgNPs was estimated to be less than 0.05% of the total film weight. Even though it was coated with a small amount of AgNPs, the PDMS film exhibited reduction of E. coli and S. aureus with values of log10 4.8 and log10 5.7, respectively. The biosafety of the AgNP-attached PDMS film was examined by contact of cells with the film or film eluent. Counting of viable cells revealed no significant cytotoxicity of the in situ-fabricated AgNPs on the PDMS film.
Since the first use of a silicone elastomer tube for duct repair in biliary surgery 60 years ago, silicone materials have been widely used in medical applications because of their superior biocompatibility compared with that of other materials . Notably, PDMS-based elastomers satisfy the criteria for biocompatibility, including nonirritating and nonsensitizing behaviors. Additionally, PDMS is thermally and chemically stable. These characteristics have allowed for the long-term use of PDMS-based implants [2, 3]. However, the hydrophobic nature of PDMS results in the adhesion of bacteria on the surface of these devices, leading to microbial infections. In the United States, more than 250,000 primary blood stream infections occur annually among 150 million intravascular devices . Antibacterial properties of medical devices can be achieved by coating the surface or mixing a PDMS elastomer with biocides, such as antibiotics, silver ion, furanones, or 3-(trimethoxysilyl)-ropyldimethyloctadecylammonium chloride . Among reported bacterial killing agents, silver nanoparticles (AgNPs) are attractive because they show unique properties such as long-term stability and broad antibacterial activities . AgNP—coated implantable medical devices such as catheters, prosthetics, bone adhesives, contact lenses, and ureteral stents have shown promising results that support the use of AgNPs as potential antibacterial agents in such devices [7–10]. Several methods to fabricate polymer–nanoparticle composites have been reported, such as mixing AgNPs with elastomers , immobilization of AgNPs on the surface of polymers , and synthesizing AgNPs inside of elastomers . The silver ions released from AgNPs play key roles in such systems demonstrating antibacterial effects. Since most AgNPs mixed with elastomers should not be exposed to the external environment, a small number of mixed AgNPs were used as antibacterial agents. Therefore, immobilizing methods are more effective than mixing methods. However, immobilizing methods are more complex and expensive than mixing methods because of the additional conjugating or layer-by-layer chemistry between the surface of polymers and AgNPs [11, 12]. Herein, we present a method to synthesize AgNPs on the surface of PDMS. An easy and facile process for the in situ fabrication of nanoparticles with no further conjugating chemistry for the polymer or nanoparticle is reported. Effective antibacterial activity of the nanocomposites against both E. coli and S. aureus was achieved. Additionally, no cellular toxicity of the nanocomposites was observed.
Silver nitrate (AgNO3, 99%), sodium hydroxide, hydrochloric acid, sodium chloride, yeast extract, d-glucose, meat extract, Mueller–Hinton broth (MHB), 3-(4,5-dimethylthiazol-2-yl)-2,5-diphenyltetrazoliumbromide (MTT), and sodium citrate (99%) were purchased from Sigma-Aldrich. Polydimethylsiloxane (MED-664) was purchased from Nusil. Acetone, isopropanol, and ethanol were obtained from Merck. Peptone, beef extract agar powder, Eagle’s minimum essential medium (EMEM), and tryptone were purchased form BD Difco. Fetal bovine serum (FBS) was purchased from Fisher Scientific. For antibacterial tests, E. coli (ATCC 8739) and S. aureus (ATCC 6538P) were used. Cytotoxicity effects mediated by the PDMS film were tested using fibroblast cells.
The PDMS film was fabricated according to the manufacturer’s instructions. In brief, part A and B of the kit were mixed thoroughly at a ratio of 1:1 by weight using an up-stirrer (IKA), and the mixture was then degassed under vacuum to remove any entrapped air bubble. The homogeneous mixture was uniformly dispersed on a Teflon film coated plate, and then was cured at 60 °C for 16–18 h under vacuum. The pre-cured PDMS film was cured at 120 °C for 1 h followed by additional curing at 150 °C for another 1 h. Unreacted elastomers and solvent were removed by successive rounds of ultrasonic cleaning of the cured film in acetone, isopropanol and distilled water, respectively, for 30 min per wash. This cleaning step was repeated two more times.
To synthesize AgNPs on the the PDMS films, the films underwent air plasma treatment in a 18W plasma cleaner (PDC-32G-2, Harrick Plasma) for 10 min under vacuum. To form Ag seeds on the film, immediately after the plasma treatment the PDMS films were immersed in 150 ml AgNO3 (10 mM) solution at room temperature for 1 h, followed by the addition of 3 ml NaBH4 (50 mM) solution and incubation for 15 min. To grow Ag seeds, the PDMS film in 150 ml 0.0167% AgNO3 was heated to 80 °C, followed by the injection of 3 ml 1% (by weight) sodium citrate (Sigma-Aldrich) as a reducing agent of silver ions. After injecting sodium citrate, the color of the solution that contained the PDMS film turned to brown within 5 min. The AgNP growth reaction was incubated for 2 h and repeated once or twice as needed. Residues on the film, such as the organic solvent from the elastomers, were removed by ultrasonic cleaning, as described above. The formation of AgNPs on the PDMS films was monitored by measuring the absorbance spectra of the film with a UV–Vis–NIR spectrometer (Agilent Technologies, Cary 5000). The size and shape of the AgNPs were investigated by imaging the films using a scattering emission microscope (Hitachi SU8010). The amount of AgNPs on the film was analyzed with an inductively coupled plasma mass spectrometer (Agilent ICP-MS 7700S).
To determine the optimal number of rounds of the AgNP growth reaction, antibacterial activity was determined by spraying E. coli cultures on a PDMS film and measuring the numbers of colonies on the film . First, a 100 ml aliquot of a bacterial suspension in PBS (~ 1011 cells per ml) that had been stored at − 20 °C was thawed at room temperature. The bacterial suspension was added to a sterile 50 ml centrifuge tube that contained 20 ml yeast dextrose broth and was shaken at 200 rpm at 20 °C overnight. The next day, the bacterial suspension was centrifuged at 6000 rpm (11,470×g) at room temperature for 10 min, and the bacterial pellet was resuspended in 20 ml PBS and vortexed for 2 min; this step was repeated once more. The harvested bacterial cells were diluted in PBS to a final concentration of 5 × 107 cells per ml by measuring the OD of the bacterial suspension at 540 nm (an OD value of ~ 1 indicates 109 bacterial cells per ml). The diluted bacterial suspensions were sprayed onto a PDMS film at a rate of ~ 10 ml min−1 by adjusting the air flow with a chromatography sprayer. Films were air dried for 2 min at room temperature and placed in a Petri dish covered with solid growth agar (25 × 75 mm2) followed by incubation of the Petri dish after sealing with Parafilm at 37 °C overnight. Colonies that had grown on the tested film were then compared. The reduction in bacterial growth by the AgNP-grown PDMS film was estimated according to a modified version of ISO 22196, a protocol for measuring the antimicrobial activity of plastic surfaces . A total of 10 ml MHB was inoculated and cultured overnight at 37 °C in a shaker. On the day of the test, 200 μl of the overnight culture was grown in 10 ml fresh MHB and shaken at 37 °C for 1 h to achieve exponential growth. The 1 h culture was diluted with saline using a spectrophotometer to achieve a cell density of 107 colony forming units (CFU) ml−1. Each film surface was inoculated with 50 μl 107 CFU ml−1 culture and covered with a polyethylene film to prevent drying of the inoculated culture. Each film was incubated at room temperature in a Petri dish sealed with Parafilm containing pieces of paper saturated with water to avoid drying of the test surface. Bacterial growth after 24 h of inoculation was determined by transferring the film to a 50-ml conical tube filled with 10 ml 0.9% sodium chloride solution, which was stirred for 30 s to recover the inoculum. Finally, 1 ml of the resulting solution was serially diluted, plated on Mueller–Hinton agar, and incubated at 37 °C for 24 h to determine the final CFU. The log10 reduction was calculated from the initial inoculum by subtracting the log10 count from the control assay on the test surface.
Biological safety of the AgNP-fabricated on PDMS film was examined with the MTT assay using the film elute and direct contact of the film to the tested cells (fibroblast cells). The MTT assay was carried out according to ISO 1093-5 . The PDMS film elute was prepared by immersing the PDMS film (25 × 75 mm2) in 20 ml EMEM that contained 10% FBS and 1× antibiotic. Cells were exposed to the material elute or allowed to contact sterilized PDMS film (10 × 10 mm2) for 24 h. For the control group, 105 cells were cultured for 24 h, and then were cultured in fresh EMEM without serum for another 24 h. Cell viability was determined using the MTT assay. The MTT solution was prepared at 1 mg ml−1 in complete medium immediately prior to use. Then, 0.6 ml MTT solution was added to each well, and cells were incubated in a humidified atmosphere of 5% CO2 at 37 °C for 4 h. After the incubation period, supernatant was removed and dark blue formazan crystals that had formed were dissolved in 0.6 ml ethanol. Plates were shaken for 5 min and then the blue solution was transferred to a 96-well plate; optical densities were read at 570 nm in a multiwell spectrophotometer (TECAN Infinite® 200).
3 Results and discussion
In the present study, we successfully demonstrated the in situ synthesis of AgNPs on the PDMS film for use as an antibacterial surface. The AgNP–PDMS composite showed high antibacterial activity against representative infectious bacterial growth. Of the total weight of the film, a small amount was represented by silver. Since all of the AgNPs were placed on the surface of PDMS film, they (~ only 0.048% of the total weigh of the PDMS film) could act to prevent bacterial growth, resulting in effective antibacterial activity. The oxidative release of Ag+ from Ag0 NP is known to drive antibacterial actions, such as binding to a wide variety of targets that contain organic amines, phosphates, thiol-containing proteins, and DNA, and can increase reactive oxygen species and simultaneously perturb many aspects of the cell metabolism . Thus, the release of silver ions can negatively impact the surrounding cells via similar antibacterial actions. Therefore, it is crucial to minimize the cytotoxicity of the antibacterial surface while maintaining its bacterial killing activity. There are several ways to avoid the side effects of AgNPs for uses in medical applications, such as the layer-by-layer technique  and plasma immersion ion implantation , to prepare AgNP-containing antibacterial polymer films. In a comparison of these methods, the in situ synthesis of AgNPs on the PDMS film presented herein is straightforward and less dependent on instruments. Consequently, it could be easily integrated in the existing manufacturing process of PDMS-based medical devices. Goyal et al. reported an in situ synthesis of AgNP inside of the PDMS film by mixing silver precursors with elastomers and then reducing them . Since most AgNPs were embedded in the film, only 80 and 52% reduction growth of E. coli and B. subtilis, respectively, was reported. By contrast, we achieved more than a five log10 reduction of bacteria with a small amount of AgNPs because all AgNPs synthesized in present study were located on the film surface. We believe that our finding could be useful for manufacturing a silicone-based implanting device with antibacterial activity by proving the straightforward and price economically competitive method.
All authors have contributed to the writing of the manuscript. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
This study was supported by a Grant of the Daegu-Gyeongbuk Medical Innovation Foundation Medical Device Development Center R&D Project (DG13D001).
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- H.E. Pearse, Ann. Surg. 124, 1020 (1946)View ArticleGoogle Scholar
- A.J. Domb, Khan W (eds.), Focal Controlled Drug Delivery (Springer, Boston, MA, 2014)Google Scholar
- A. Colas, J Curtis, in Silicone Biomaterials: History and Chemistry & Medical Applications of Silicones, 2nd edn, ed. By B.D. Ratner, A.S. Hoffman, F.J. Schoen, J.E. Lemons (Elsevier, Amsterdam, 2004)Google Scholar
- D.G. Maki, D.M. Kluger, C.J. Crnich, Mayo Clin. Proc. 81, 1159 (2006)Google Scholar
- M. Chen, Q. Yu, H. Sun, Int. J. Mol. Sci. 14, 18488 (2013)View ArticleGoogle Scholar
- B. Le Ouay, F. Stellacci, Nano Today 10, 339 (2015)View ArticleGoogle Scholar
- P.A. Gunatillake, D.J. Martin, G.F. Meijs, S.J. McCarthy, R. Adhikari, Aus. J. Chem. 56, 545 (2003)View ArticleGoogle Scholar
- Z.M. Davoudi, A.E. Kandjani, A.I. Bhatt, I.L. Kyratzis, A.P. O’Mullane, V. Bansal, Adv. Funct. Mater. 24, 1047 (2014)View ArticleGoogle Scholar
- M.D. Willcox, E.B. Hume, A.K. Vijay, R. Petcavich, J. Optom. 3, 143 (2010)View ArticleGoogle Scholar
- C. Tieszer, G. Reid, J. Denstedt, J. Biomed. Mater. Res. A. 43, 321 (1998)View ArticleGoogle Scholar
- S. Huda, S.K. Smoukov, H. Nakanishi, B. Kowalczyk, K. Bishop, B.A. Grzybowski, A.C.S. Appl, Mater. Interfaces 2, 1206 (2010)View ArticleGoogle Scholar
- S.N. Sawant, V. Selvaraj, V. Prabhawathi, M. Doble, PLoS ONE 8, e63311 (2013)View ArticleGoogle Scholar
- A. Goyal, A. Kumar, P.K. Patra, S. Mahendra, S. Tabatabaei, P.J. Alvarez, G. John, P.M. Ajayan, Macromol. Rapid Comm. 30, 1116 (2009)View ArticleGoogle Scholar
- J. Haldar, A.K. Weight, A.M. Klibanov, Nat. Protoc. 2, 2412 (2007)View ArticleGoogle Scholar
- ISO 22196:2007, Plastics—Measurement of antibacterial activity on plastics surfaces, 1st edn, International Standard (2007)Google Scholar
- ISO 10993-5, Biological evaluation of medical devices—Part 5: Tests for in vitro cytotoxicity, 3rd edn, International Standard (2009)Google Scholar
- J.F. Gomes, A.C. Garcia, E.B. Ferreira, C. Pires, V.L. Oliveira, G. Tremiliosi-Filho, L.H. Gasparotto, Phys. Chem. Chem. Phys. 17, 21683 (2015)View ArticleGoogle Scholar
- Q. Bao, D. Zhang, P. Qi, J. Colloid Interf. Sci. 360, 463 (2011)View ArticleGoogle Scholar
- P. Zhang, Y. Huang, X. Lu, S. Zhang, J. Li, G. Wei, Z. Su, Langmuir 30, 8980 (2014)View ArticleGoogle Scholar
- S.K. Sia, G.M. Whitesides, Electrophoresis 24, 3563 (2003)View ArticleGoogle Scholar
- B.T. Ginn, O. Steinbock, Langmuir 19, 8117 (2003)View ArticleGoogle Scholar
- A. Agarwal, K.M. Guthrie, C.J. Czuprynski, M.J. Schurr, J.F. McAnulty, C.J. Murphy, N.L. Abbott, Adv. Funct. Mater. 21, 1863 (2011)View ArticleGoogle Scholar
- W. Zhang, Y. Luo, H. Wang, J. Jiang, S. Pu, P.K. Chu, Acta Biomater. 4, 2028 (2008)View ArticleGoogle Scholar